Published on

18-Aug-2016View

213Download

1

Embed Size (px)

Transcript

<ul><li><p>PRAMANA __ journal of </p><p>physics </p><p> Printed in India Vol. 47, No. 6, December 1996 pp. 447-470 </p><p>A stochastic model for solidification I. The basic equations, their analysis and solution </p><p>SHOBHA DASS, GAUTAM JOHRI* and LAKSHMAN PANDEY* Govt. M.H. College of Science and Home Science, Jabalpur 482 002, India *Department of Post Graduate Studies and Research in Physics, Rani Durgavati University, Jabalpur 482 001, India </p><p>MS received 4 April 1995; revised 8 November 1995 </p><p>Abstract. A 3-dimensional (2-space, 1-time) model relating the diffusion of heat and mass to the kinetic processes at the solid-liquid interface, using a stochastic approach is presented in this paper. This paper is divided in two parts. In the first part the basic set of equations describing solidification alongwith their analysis and solution are given. The process of solidification has a stochastic character and depends on the net probability of transfer of atoms from liquid to the solid phase. This has been modeled by a Markov process in which knowledge of the parameters at the initial time only is needed to evaluate the time evolution of the system. Solidification process is expressed in terms of four coupled equations, namely, the diffusion equations for heat and mass, the equations for concentration of the solid phase and for rate of growth of the solid-liquid interface. The position of the solid-liquid interface is represented with the help of a delta function and it is defined as the surface at which latent heat is evolved. A numerical method is used to solve the equations appearing in the model. In the second part the results i.e. the time evolution of the solid-liquid interface shape and its concentration, rate of growth and temperature are given. </p><p>Keywords. Stochastic; solidification; binary melt; kinetic phase diagrams. </p><p>PACS No. 81.10 </p><p>1. Introduction </p><p>Solidification and melting are the types of phenomenon commonly observed during the production of materials. Most of the materials undergo a process of melting and solidification during their manufacture. Some of the typical manufacturing processes are casting, welding, melt spinning, surface remelting and directional solidification process for growing crystals using Bridgman, Czochralski and Electroslag remelting techniques [1, 2,1. In all these techniques the basic objective is to maintain external conditions such that a crystal with desired and reproducible properties is obtained. </p><p>Processes such as rapid solidification, directional solidification or surface alloying are often used to create new materials or impart new properties to the existing ones. Many of the production processes of high-tech materials such as high temperature superconductors, magnetic materials, ceramics, composites etc. involve application of high cooling rates and large changes of pressures [8,1. Such conditions render these processes far from thermodynamical equilibrium and lead to various metastable states of these materials, for example quasicrystals [3, 41, metallic glasses etc. [5-7,1, with diverse new properties. Also, properties of materials are governed to a large extent by their microstructure which in turn is greatly influenced by the solidification process. </p><p>447 </p></li><li><p>Shobha Dass et al </p><p>Therefore a correlation between solidification parameters and the resulting micro- structure is of utmost importance for producing materials having tailormade properties. A qualitative information about this can be obtained by performing a series of experiments by using different solidification parameters. However, the experimentation is quite tedious and crystal defects are difficult to eliminate once they are created. Therefore solidification phenomenon has received considerable theoretical attention with a view to be able to model the process and predict the microstructure and hence the properties. </p><p>The existing theories treat solidification process as the one involving nucleation and growth [8-11]. The phenomenological thermodynamics deals with the conditions of phase transformation and the equilibrium co-existence of phases and facilitates the construction of equilibrium phase diagrams [1, 12, 13]. These phase diagrams are often used to predict the constitution of the phases during the solidification of materials, even though their employment is questionable as during solidification the system may be far from thermodynamic equilibrium. Therefore the study of the dynamics of metastable and unstable states becomes essential for a controlled synthesis of new materials with desired and reproducible properties. </p><p>Among the modern theories which deal with nucleation process are the stochastic theory [-9, 10], the renormalization group method [14] and the field theories [15-17]. However, the kinetics of phase transformation were neglected in all these models. The study of phase transformation kinetics was also developed using other theories such as spinodal decomposition theory [18], the molecular dynamics method [8, 19], the functional density method [20, 21] and the fractal geometry method [22, 23]. The molecular dynamics method [8, 19] is too demanding in terms of computational time. In functional density method [20, 21] the structure of the solid phase is assumed to be known and temperature is taken to be a constant. Fractal geometry method [22, 23] also assumes the structure of the solid phase. </p><p>Nonequilibrium thermodynamics was used by Caroli et al [24] to study solidifica- tion. Some other calculations of the non stationary solidification process have been done based on the Monte Carlo method [25], where growth of only 20 atomic layers was simulated. The concept of kinetic phase diagrams was developed by Cherepanona ['26, 27] to describe processes where equilibrium phase diagrams can not be used. In these models constant temperature and concentration was assumed at the interface. </p><p>Kinetic phase transformation theories have been formulated dealing with the formation of a new phase (nucleation), growth of the interface and mass and energy transport in the system. In order to predict the structure and properties of materials produced by nonequilibrium experimental conditions under given initial and bound- ary conditions, a theory must be constructed which takes into account all aspects of phase transformation. Considerable efforts have been made in the past to understand the solidification process of alloys by proposing models which involve heat and mass transfer and shape of the solid-liquid interface [2, 28-30]. From the survey of literature it seems that a treatment of the solidification process taking into account its stochastic nature has not been done except by Chvoj [31-40]. Chvoj I-31-40] has proposed a stochastic model by considering the transport of heat and mass simulta- neously with the kinetic processes at the phase interface. However, he has not </p><p>448 Pramana - J. Phys., Voi. 47, No. 6, December 1996 </p></li><li><p>A stochastic model for solidification: I </p><p>considered interdependence of heat and mass flow and also has not solved the time evolution of a binary system in three dimensions (2-space, 1-time). which is closer to the real experimental situations. </p><p>In this paper a three dimensional (2-space, 1-time) stochastic mathematical model to describe the solidification phenomenon of binary melt taking into account the kinetic processes at the solid-liquid interface is proposed. This model is quite general in nature and can be applied to any material ranging from organic substances to metallic glasses. A preliminary report of the scheme of the model was presented earlier 141]. </p><p>2. The model </p><p>A solid can be grown from the melt if the melt is below its equilibrium melting temperature. Departure from the equilibrium is always required for the solidification process to proceed. Processes responsible for the formation of a solid from the melt are: thermal and density fluctuations governed by stochastic laws, diffusion of mass and heat, evolution of latent heat at the solid-liquid interface, kinetic processes at the interface, convection, radiation and initial and boundary conditions. A stochastic mathematical model has been developed to describe this phenomenon as follows. </p><p>The diffusion of mass and heat have been represented with the help of partial differential equations, derived by application of the law of conservation of mass and heat. These equations govern the distribution of mass and heat in the three regions, namely, the solid, the liquid and the solid-liquid interface. The effect of other factors such as latent heat, external fields etc. can also be included in these equations. For the description of the effect of thermodynamic fluctuations in temperature and concentra- tion, Langevin method 142] of stochastic differential equations has been used. </p><p>Kinetic processes at the solid-liquid interface have been modeled using a micro- scopic description of the process of solidification i.e. by assigning probabilities to individual atoms as they make transition from a liquid-like configuration to a solid-like configuration, and then averaging over the corresponding phases to determine the probability of formation of the new phase. </p><p>In the solidification process the dominant forces are due to temperature and concentration gradients, which give rise to heat and mass diffusion. The diffusion equations for mass and heat under non steady state growth conditions can be written as </p><p>OCt, y, t) dt = DcV2 CL(x' y' t) -t- DCT V2 T(x, y, t) + R.VCL(x, y, t) (1) </p><p>and </p><p>T(x,Y ,0 ~t : DTcVZCL(X" y' t) + DT V2 T(x, y, t) + R.VT(x, y, t) (2) </p><p>respectively, where CL is the relative concentration of B atoms in A-B system, T is the temperature of the melt, D r = k/Cvp is the diffusivity in which Cv is the volume specific heat and p is the density of the solid, D c is the diffusion coefficient, Dcr and Drc are related to the Onsager's coefficients due to interdependence of mass and heat flow, x and y are space coordinates, t is the time coordinate. Solidification process is </p><p>Pramana - J. Phys., Vol. 47, No. 6, December 1996 449 </p></li><li><p>Shobha Dass et al </p><p>considered in the x-y plane. This implies an infinite extent of the melt in the z direction and complete translational symmetry. R is the rate of growth of the solid phase, x is the direction of growth and y is the coordinate perpendicular to it. </p><p>Solidification phenomenon is brought about by a process of heat transfer that is accompanied by a change of phase i.e. from liquid to solid phase. During the phase change, thermal energy is released or absorbed at the solid-liquid interface in the form of latent heat of fusion. For solidification this heat must be drawn from liquid phase at the interface and conducted away through the solid phase. Under certain circumstan- ces, however, the liquid may not remain stagnant and essentially conductive heat transfer may be superimposed with convective heat transfer. This leads to an interface motion coupled nonlinearly to the local temperature field which obeys the diffusion law. Loss of energy can also take place by radiation from the walls of the container of the freezing material. In binary systems the composition of the new phase is different from that of the old phase. The change in composition is governed by the flux boundary condition at the solid-liquid interface. Heat and mass can be produced by chemical reactions also. Solidification process can also be affected by the presence of external fields, for example electric, magnetic or acoustic fields. Finally fluctuations of ther- modynamic quantities such as temperature and concentration also contribute to a change in mass and energy of the system. Taking these factors into account the diffusion equations (1) and (2) can be written as </p><p>Ot = DcV2CL(X' y' t) + DcrV 2 T(x, y, t) + R.VCdx, y, t) </p><p>and </p><p>+ div F c + div E c + Qc (3) </p><p>TIX, y ,t) </p><p>gt = DTcV2C~(x' y' t) + DrV 2 T(x, y, t) + R.VT(x, y, t) </p><p>+ div F r + div E r + Qr, (4) </p><p>where Qr and Qc are respectively the heat and mass produced clue to phase transform- ation, Er and E c are the heat and mass flux controlled by external fields, respectively, Fr and Fc are the stochastic terms that represent the flux of heat and mass clue to fluctuations, respectively. </p><p>The effect of convection and radiation is not included in this model. Also diffusion in the solid phase, effect of capillarity at the solid-liquid interface and change of volume during phase transformation are neglected. The source terms Qc and Qr appearing due to the change of phase, at the interface can be expressed as [39] </p><p>Qc = Qc 6(x - X,(y, t)), (5) where </p><p>~ = (c~, - C~, )R (6) and </p><p>(7) AR </p><p>QT = ~ 6(x - XrtY, t)), CvP </p><p>450 Pramana - J. Phys., Vol. 47, No. 6, December 1996 </p></li><li><p>A stochastic model for solidification: I </p><p>where Cs, and CL, are the solid and liquid concentrations at the interface X,(t), respectively, A is the latent heat per unit volume. </p><p>Equations (3) and (4) are the stochastic differential equations representing the time evolution of temperature and liquid concentration. For evaluation of the fluctuation terms F r and F c the Langevin method of stochastic differential equations has been used [39, 42]. According to this method the average of the random fluctuations is taken equal to zero and it can be written as </p><p>(F t . c(X, t)) = 0 </p><p>and for t ~ t', x ~ x', the fluctuations Fr.c(X,t ) and Fr, c(X',t' ) are statistically independent. Mathematically this can be expressed as </p><p>(Fr,c(X, t) FT,c(X', t ')) = Krc(X, t) Ix -- x ' ] fi Et -- t ' ] and thus </p><p>(div F r ) = (div Fc) = 0, </p><p>which is characteristic of the Markov process. The function Krc(X, t) can be derived from the microscopic models. The effect of external fields other than thermal field is considered to be negligible i.e. E c = E r = O. </p><p>In order to solve equations (3) and (4), the average rate of growth of the solid-liquid interface must be determined. This can be determined by evaluating probability density of formation of a new monoatomic layer. This probability can be obtained by considering the microscopic processes of atom transfer from one phase to the other at the interface. </p><p>2.1 Calculation of growth rate and solid concentration </p><p>Atoms arriving at the sohd-liquid interface can make transition to the other phase depending on their activation energies. The number of possible transitions of one B atom from the liquid to the solid phase across the interface per unit time is given by [39] </p><p>NS _ . L..L B - - VB "B ' (8 ) </p><p>where n s = CLrfl L is the number of B atoms in a monoatomic layer at the interface in the liquid phase, pL is the total number of atoms per unit volume in a monoatomic layer at the interface in the liquid phase. </p><p>Similarly, the number of possible transitions of one A atom from the liquid to the solid phase across the interface per unit time is </p><p>N s = VLA nLA, (9) where </p><p>n L -- [1 - - CLr]ff L. </p><p>The corresponding numbers of B and A atoms making a transition from the solid to the liquid phase are give...</p></li></ul>